# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_pnnm_a
_database_code_depnum_ccdc_archive 'CCDC 2244533'
loop_
_audit_author_name
_audit_author_address
'Yingjie Zhang'
;Australian Nuclear Science and Technology Organisation
Australia
;
_audit_update_record             
;
2023-02-25 deposited with the CCDC.	2023-04-25 downloaded from the CCDC.
;
_audit_creation_date             2023-02-25
_audit_creation_method           
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cd3 K2 O22 U6, O'
_chemical_formula_sum            'Cd3 K2 O23 U6'
_chemical_formula_weight         2211.58
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           58
_space_group_name_H-M_alt        'P n n m'
_space_group_name_Hall           '-P 2 2n'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'x-1/2, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   12.398(3)
_cell_length_b                   7.0070(14)
_cell_length_c                   11.482(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     997.5(3)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    16000
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      25.999
_cell_measurement_theta_min      2.41
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    52.169
_exptl_absorpt_correction_T_max  0.4343
_exptl_absorpt_correction_T_min  0.2814
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.1842 before and 0.0548 after correction.
The Ratio of minimum to maximum transmission is 0.6479.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    7.363
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             1836
_exptl_crystal_size_max          0.050
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.005
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0569
_diffrn_reflns_av_unetI/netI     0.0243
_diffrn_reflns_Laue_measured_fraction_full 0.991
_diffrn_reflns_Laue_measured_fraction_max 0.991
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            12530
_diffrn_reflns_point_group_measured_fraction_full 0.991
_diffrn_reflns_point_group_measured_fraction_max 0.991
_diffrn_reflns_theta_full        25.244
_diffrn_reflns_theta_max         25.998
_diffrn_reflns_theta_min         2.418
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_radiation_type           
'silicon double crystal monochromated synchrotron'
_diffrn_source                   'Australian Synchrotron MX2'
_diffrn_measurement_device_type  'Eiger Detector'
_diffrn_measurement_method       'π  scans'
_diffrn_radiation_wavelength     0.71078
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                999
_reflns_number_total             1028
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_data_collection       'BlueIce (McPhillips, et al., 2002)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         2.494
_refine_diff_density_min         -3.446
_refine_diff_density_rms         0.473
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.081
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     79
_refine_ls_number_reflns         1028
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0300
_refine_ls_R_factor_gt           0.0294
_refine_ls_restrained_S_all      1.081
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0411P)²+31.3277P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0814
_refine_ls_wR_factor_ref         0.0822
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O5) = Uanis(O6) = Uanis(O7)
2. Others
 Fixed Sof: Cd2(0.25)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.24312(4) 0.18673(7) 0.500000 0.00744(19) Uani 1 2 d S T P . .
U2 U 0.24322(3) 0.68256(6) 0.31773(4) 0.00765(17) Uani 1 1 d . . . . .
Cd1 Cd 0.500000 1.000000 0.35208(8) 0.0091(2) Uani 1 2 d S T P . .
Cd2 Cd 0.000000 0.500000 0.4757(2) 0.0478(11) Uani 0.5 2 d S T P . .
K1 K 0.000000 1.000000 0.3235(4) 0.0334(10) Uani 1 2 d S T P . .
O1 O 0.0872(9) 0.2440(15) 0.500000 0.021(2) Uani 1 2 d S T P . .
O2 O 0.3987(7) 0.1136(14) 0.500000 0.0139(19) Uani 1 2 d S T P . .
O3 O 0.2193(6) 0.0024(9) 0.3551(6) 0.0106(13) Uani 1 1 d . . . . .
O4 O 0.2690(6) 0.3646(11) 0.3537(6) 0.0136(14) Uani 1 1 d . . . . .
O5 O 0.0948(6) 0.6350(10) 0.2973(6) 0.0145(9) Uani 1 1 d . . . . .
O6 O 0.3900(6) 0.7297(10) 0.3335(5) 0.0145(9) Uani 1 1 d . . . . .
O7 O 0.2117(8) 0.6670(13) 0.500000 0.0145(9) Uani 1 2 d S T P . .
O8 O 0.500000 0.500000 0.500000 0.023(4) Uani 1 4 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 U2 3.6523(9) 8_656 ?
U1 U2 3.6523(9) 3_545 ?
U1 Cd2 3.7393(8) . ?
U1 Cd2 3.7393(8) 5_566 ?
U1 K1 3.861(2) 1_545 ?
U1 K1 3.861(2) 5_566 ?
U1 O1 1.974(11) . ?
U1 O2 1.996(9) . ?
U1 O3 2.127(6) . ?
U1 O3 2.127(6) 6_556 ?
U1 O4 2.116(7) 6_556 ?
U1 O4 2.116(7) . ?
U2 U2 3.8369(8) 3 ?
U2 Cd2 3.7440(14) . ?
U2 K1 3.7476(7) . ?
U2 K1 3.7948(19) 3_545 ?
U2 O3 2.301(7) 1_565 ?
U2 O3 2.397(7) 3 ?
U2 O4 2.350(8) 3 ?
U2 O4 2.289(8) . ?
U2 O5 1.885(7) . ?
U2 O6 1.858(7) . ?
U2 O7 2.132(2) . ?
Cd1 Cd1 3.397(2) 5_676 ?
Cd1 K1 4.042(2) 3_545 ?
Cd1 K1 4.042(2) 3 ?
Cd1 O2 2.257(6) 1_565 ?
Cd1 O2 2.257(6) 5_666 ?
Cd1 O5 2.284(7) 4_565 ?
Cd1 O5 2.284(7) 3 ?
Cd1 O6 2.344(7) 2_675 ?
Cd1 O6 2.344(7) . ?
Cd2 Cd2 0.559(5) 5_566 ?
Cd2 K1 3.915(2) . ?
Cd2 K1 4.194(3) 5_576 ?
Cd2 K1 3.915(2) 1_545 ?
Cd2 O1 2.113(11) . ?
Cd2 O1 2.113(11) 5_566 ?
Cd2 O5 2.544(7) 2_565 ?
Cd2 O5 2.544(7) . ?
K1 O1 2.864(8) 5_566 ?
K1 O1 2.864(8) 1_565 ?
K1 O3 2.743(7) 1_565 ?
K1 O3 2.743(7) 2_565 ?
K1 O5 2.830(7) . ?
K1 O5 2.830(7) 2_575 ?
K1 O6 2.775(7) 4_465 ?
K1 O6 2.775(7) 3 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
U2 U1 U2 174.60(2) 8_656 3_545 ?
U2 U1 Cd2 88.14(4) 3_545 . ?
U2 U1 Cd2 96.70(4) 3_545 5_566 ?
U2 U1 Cd2 96.70(4) 8_656 . ?
U2 U1 Cd2 88.14(4) 8_656 5_566 ?
U2 U1 K1 60.60(5) 3_545 1_545 ?
U2 U1 K1 123.91(6) 3_545 5_566 ?
U2 U1 K1 60.60(5) 8_656 5_566 ?
U2 U1 K1 123.91(6) 8_656 1_545 ?
Cd2 U1 Cd2 8.57(8) . 5_566 ?
Cd2 U1 K1 66.97(3) 5_566 1_545 ?
Cd2 U1 K1 61.99(3) 5_566 5_566 ?
Cd2 U1 K1 66.97(3) . 5_566 ?
Cd2 U1 K1 61.99(3) . 1_545 ?
K1 U1 K1 63.34(11) 1_545 5_566 ?
O1 U1 U2 92.696(10) . 8_656 ?
O1 U1 U2 92.696(10) . 3_545 ?
O1 U1 Cd2 24.7(3) . . ?
O1 U1 Cd2 24.7(3) . 5_566 ?
O1 U1 K1 45.9(2) . 5_566 ?
O1 U1 K1 45.9(2) . 1_545 ?
O1 U1 O2 176.8(4) . . ?
O1 U1 O3 89.3(3) . . ?
O1 U1 O3 89.3(3) . 6_556 ?
O1 U1 O4 91.7(3) . . ?
O1 U1 O4 91.7(3) . 6_556 ?
O2 U1 U2 87.313(10) . 3_545 ?
O2 U1 U2 87.313(10) . 8_656 ?
O2 U1 Cd2 158.4(3) . . ?
O2 U1 Cd2 158.4(3) . 5_566 ?
O2 U1 K1 131.9(2) . 1_545 ?
O2 U1 K1 131.9(2) . 5_566 ?
O2 U1 O3 88.8(3) . . ?
O2 U1 O3 88.8(3) . 6_556 ?
O2 U1 O4 90.3(3) . . ?
O2 U1 O4 90.3(3) . 6_556 ?
O3 U1 U2 38.75(18) . 3_545 ?
O3 U1 U2 141.54(18) . 8_656 ?
O3 U1 U2 38.75(18) 6_556 8_656 ?
O3 U1 U2 141.54(18) 6_556 3_545 ?
O3 U1 Cd2 107.64(18) 6_556 . ?
O3 U1 Cd2 100.72(18) 6_556 5_566 ?
O3 U1 Cd2 107.64(18) . 5_566 ?
O3 U1 Cd2 100.72(18) . . ?
O3 U1 K1 95.5(2) 6_556 1_545 ?
O3 U1 K1 43.54(19) 6_556 5_566 ?
O3 U1 K1 43.54(19) . 1_545 ?
O3 U1 K1 95.5(2) . 5_566 ?
O3 U1 O3 102.9(4) 6_556 . ?
O4 U1 U2 37.3(2) . 3_545 ?
O4 U1 U2 142.3(2) 6_556 3_545 ?
O4 U1 U2 142.3(2) . 8_656 ?
O4 U1 U2 37.3(2) 6_556 8_656 ?
O4 U1 Cd2 80.56(19) 6_556 . ?
O4 U1 Cd2 73.58(19) 6_556 5_566 ?
O4 U1 Cd2 80.56(19) . 5_566 ?
O4 U1 Cd2 73.58(19) . . ?
O4 U1 K1 137.3(2) 6_556 1_545 ?
O4 U1 K1 84.3(2) . 1_545 ?
O4 U1 K1 137.3(2) . 5_566 ?
O4 U1 K1 84.3(2) 6_556 5_566 ?
O4 U1 O3 76.0(3) 6_556 6_556 ?
O4 U1 O3 76.0(3) . . ?
O4 U1 O3 178.5(3) . 6_556 ?
O4 U1 O3 178.5(3) 6_556 . ?
O4 U1 O4 105.1(4) 6_556 . ?
U1 U2 U2 65.526(15) 3 3 ?
U1 U2 Cd2 121.60(4) 3 . ?
U1 U2 K1 92.87(7) 3 . ?
U1 U2 K1 62.42(6) 3 3_545 ?
Cd2 U2 U2 122.932(16) . 3 ?
Cd2 U2 K1 63.02(4) . . ?
Cd2 U2 K1 140.12(2) . 3_545 ?
K1 U2 U2 60.03(3) . 3 ?
K1 U2 U2 95.61(3) 3_545 3 ?
K1 U2 K1 151.960(16) . 3_545 ?
O3 U2 U1 100.63(16) 1_565 3 ?
O3 U2 U1 33.73(16) 3 3 ?
O3 U2 U2 36.09(16) 1_565 3 ?
O3 U2 U2 97.86(16) 3 3 ?
O3 U2 Cd2 112.16(17) 3 . ?
O3 U2 Cd2 97.97(18) 1_565 . ?
O3 U2 K1 46.07(17) 3 3_545 ?
O3 U2 K1 46.76(17) 1_565 . ?
O3 U2 K1 118.88(17) 3 . ?
O3 U2 K1 121.07(18) 1_565 3_545 ?
O3 U2 O3 133.80(18) 1_565 3 ?
O3 U2 O4 67.6(2) 1_565 3 ?
O4 U2 U1 33.08(19) 3 3 ?
O4 U2 U1 100.45(18) . 3 ?
O4 U2 U2 33.68(18) 3 3 ?
O4 U2 U2 162.93(18) . 3 ?
O4 U2 Cd2 122.62(18) 3 . ?
O4 U2 Cd2 72.10(18) . . ?
O4 U2 K1 83.07(19) 3 3_545 ?
O4 U2 K1 133.41(18) . . ?
O4 U2 K1 68.94(19) 3 . ?
O4 U2 K1 68.38(18) . 3_545 ?
O4 U2 O3 67.0(2) . 3 ?
O4 U2 O3 66.7(3) 3 3 ?
O4 U2 O3 158.9(3) . 1_565 ?
O4 U2 O4 133.5(2) . 3 ?
O5 U2 U1 85.6(2) . 3 ?
O5 U2 U2 98.8(2) . 3 ?
O5 U2 Cd2 38.1(2) . . ?
O5 U2 K1 134.9(2) . 3_545 ?
O5 U2 K1 47.3(2) . . ?
O5 U2 O3 94.0(3) . 1_565 ?
O5 U2 O3 89.6(3) . 3 ?
O5 U2 O4 85.9(3) . 3 ?
O5 U2 O4 89.2(3) . . ?
O5 U2 O7 86.2(3) . . ?
O6 U2 U1 92.9(2) . 3 ?
O6 U2 U2 80.5(2) . 3 ?
O6 U2 Cd2 143.3(2) . . ?
O6 U2 K1 44.0(2) . 3_545 ?
O6 U2 K1 132.9(2) . . ?
O6 U2 O3 86.3(3) . 1_565 ?
O6 U2 O3 89.1(3) . 3 ?
O6 U2 O4 91.1(3) . . ?
O6 U2 O4 92.8(3) . 3 ?
O6 U2 O5 178.5(3) . . ?
O6 U2 O7 95.3(3) . . ?
O7 U2 U1 171.7(3) . 3 ?
O7 U2 U2 116.9(2) . 3 ?
O7 U2 Cd2 50.2(3) . . ?
O7 U2 K1 123.8(3) . 3_545 ?
O7 U2 K1 82.3(3) . . ?
O7 U2 O3 145.2(3) . 3 ?
O7 U2 O3 81.0(3) . 1_565 ?
O7 U2 O4 146.9(3) . 3 ?
O7 U2 O4 78.4(3) . . ?
Cd1 Cd1 K1 119.91(5) 5_676 3 ?
Cd1 Cd1 K1 119.91(5) 5_676 3_545 ?
K1 Cd1 K1 120.17(11) 3_545 3 ?
O2 Cd1 Cd1 41.20(18) 1_565 5_676 ?
O2 Cd1 Cd1 41.20(18) 5_666 5_676 ?
O2 Cd1 K1 94.0(2) 1_565 3 ?
O2 Cd1 K1 132.9(3) 5_666 3 ?
O2 Cd1 K1 132.9(3) 1_565 3_545 ?
O2 Cd1 K1 94.0(2) 5_666 3_545 ?
O2 Cd1 O2 82.4(4) 5_666 1_565 ?
O2 Cd1 O5 175.7(3) 5_666 3 ?
O2 Cd1 O5 175.7(3) 1_565 4_565 ?
O2 Cd1 O5 97.6(3) 5_666 4_565 ?
O2 Cd1 O5 97.6(3) 1_565 3 ?
O2 Cd1 O6 91.7(3) 5_666 2_675 ?
O2 Cd1 O6 91.7(3) 1_565 . ?
O2 Cd1 O6 96.2(3) 1_565 2_675 ?
O2 Cd1 O6 96.2(3) 5_666 . ?
O5 Cd1 Cd1 138.67(17) 4_565 5_676 ?
O5 Cd1 Cd1 138.67(17) 3 5_676 ?
O5 Cd1 K1 42.82(17) 4_565 3_545 ?
O5 Cd1 K1 89.11(18) 4_565 3 ?
O5 Cd1 K1 89.11(18) 3 3_545 ?
O5 Cd1 K1 42.82(17) 3 3 ?
O5 Cd1 O5 82.7(3) 3 4_565 ?
O5 Cd1 O6 88.1(2) 3 . ?
O5 Cd1 O6 88.1(2) 4_565 2_675 ?
O5 Cd1 O6 84.1(2) 3 2_675 ?
O5 Cd1 O6 84.1(2) 4_565 . ?
O6 Cd1 Cd1 95.22(16) 2_675 5_676 ?
O6 Cd1 Cd1 95.22(16) . 5_676 ?
O6 Cd1 K1 130.92(17) 2_675 3_545 ?
O6 Cd1 K1 41.78(17) . 3_545 ?
O6 Cd1 K1 130.92(17) . 3 ?
O6 Cd1 K1 41.78(17) 2_675 3 ?
O6 Cd1 O6 169.6(3) . 2_675 ?
U1 Cd2 U1 171.43(8) 5_566 . ?
U1 Cd2 U2 119.00(3) 5_566 . ?
U1 Cd2 U2 65.639(18) 5_566 2_565 ?
U1 Cd2 U2 119.00(3) . 2_565 ?
U1 Cd2 U2 65.640(18) . . ?
U1 Cd2 K1 123.96(3) 5_566 1_545 ?
U1 Cd2 K1 123.96(3) . . ?
U1 Cd2 K1 57.90(2) 5_566 5_576 ?
U1 Cd2 K1 60.53(3) 5_566 . ?
U1 Cd2 K1 116.70(4) . 5_576 ?
U1 Cd2 K1 60.53(3) . 1_545 ?
U2 Cd2 U2 122.06(7) 2_565 . ?
U2 Cd2 K1 88.91(3) . 5_576 ?
U2 Cd2 K1 58.54(3) . . ?
U2 Cd2 K1 58.54(3) 2_565 1_545 ?
U2 Cd2 K1 123.484(17) 2_565 5_576 ?
U2 Cd2 K1 95.14(5) . 1_545 ?
U2 Cd2 K1 95.14(5) 2_565 . ?
Cd2 Cd2 U1 85.72(4) 5_566 . ?
Cd2 Cd2 U1 85.72(4) 5_566 5_566 ?
Cd2 Cd2 U2 118.97(4) 5_566 . ?
Cd2 Cd2 U2 118.97(3) 5_566 2_565 ?
Cd2 Cd2 K1 116.51(7) 5_566 . ?
Cd2 Cd2 K1 56.64(6) 5_566 5_576 ?
Cd2 Cd2 K1 116.51(7) 5_566 1_545 ?
Cd2 Cd2 O1 82.41(8) 5_566 . ?
Cd2 Cd2 O1 82.41(8) 5_566 5_566 ?
Cd2 Cd2 O5 143.62(16) 5_566 . ?
Cd2 Cd2 O5 143.62(16) 5_566 2_565 ?
K1 Cd2 K1 173.16(6) 1_545 5_576 ?
K1 Cd2 K1 59.87(11) . 5_576 ?
K1 Cd2 K1 126.98(13) 1_545 . ?
O1 Cd2 U1 23.0(3) . . ?
O1 Cd2 U1 23.0(3) 5_566 5_566 ?
O1 Cd2 U1 154.3(3) . 5_566 ?
O1 Cd2 U1 154.3(3) 5_566 . ?
O1 Cd2 U2 86.7(2) . . ?
O1 Cd2 U2 100.7(3) 5_566 . ?
O1 Cd2 U2 100.7(3) . 2_565 ?
O1 Cd2 U2 86.7(2) 5_566 2_565 ?
O1 Cd2 K1 129.52(18) . 5_576 ?
O1 Cd2 K1 45.52(19) 5_566 . ?
O1 Cd2 K1 38.6(2) 5_566 5_576 ?
O1 Cd2 K1 144.9(2) 5_566 1_545 ?
O1 Cd2 K1 45.52(19) . 1_545 ?
O1 Cd2 K1 144.9(2) . . ?
O1 Cd2 O1 164.81(16) . 5_566 ?
O1 Cd2 O5 100.7(2) . . ?
O1 Cd2 O5 91.6(2) . 2_565 ?
O1 Cd2 O5 91.6(2) 5_566 . ?
O1 Cd2 O5 100.7(2) 5_566 2_565 ?
O5 Cd2 U1 84.61(16) . . ?
O5 Cd2 U1 102.37(16) 2_565 . ?
O5 Cd2 U1 84.61(15) 2_565 5_566 ?
O5 Cd2 U1 102.37(16) . 5_566 ?
O5 Cd2 U2 96.27(17) . 2_565 ?
O5 Cd2 U2 27.24(15) 2_565 2_565 ?
O5 Cd2 U2 96.27(17) 2_565 . ?
O5 Cd2 U2 27.23(15) . . ?
O5 Cd2 K1 46.19(16) . . ?
O5 Cd2 K1 88.48(17) 2_565 . ?
O5 Cd2 K1 97.59(16) . 5_576 ?
O5 Cd2 K1 88.48(17) . 1_545 ?
O5 Cd2 K1 46.19(16) 2_565 1_545 ?
O5 Cd2 K1 138.88(16) 2_565 5_576 ?
O5 Cd2 O5 72.8(3) . 2_565 ?
U2 K1 U2 61.15(2) 2_575 4_465 ?
U2 K1 U2 117.87(5) . 4_465 ?
U2 K1 U2 117.87(5) 2_575 3 ?
U2 K1 U2 61.15(2) . 3 ?
U2 K1 U2 177.99(13) . 2_575 ?
U2 K1 U2 129.41(12) 4_465 3 ?
O1 K1 U2 93.6(2) 1_565 . ?
O1 K1 U2 77.54(17) 5_566 4_465 ?
O1 K1 U2 145.1(2) 5_566 3 ?
O1 K1 U2 87.8(2) 5_566 . ?
O1 K1 U2 77.54(17) 1_565 3 ?
O1 K1 U2 87.8(2) 1_565 2_575 ?
O1 K1 U2 93.6(2) 5_566 2_575 ?
O1 K1 U2 145.1(2) 1_565 4_465 ?
O1 K1 O1 89.9(3) 1_565 5_566 ?
O3 K1 U2 142.77(14) 2_565 . ?
O3 K1 U2 152.90(17) 2_565 3 ?
O3 K1 U2 39.01(14) 2_565 4_465 ?
O3 K1 U2 142.77(14) 1_565 2_575 ?
O3 K1 U2 37.67(14) 2_565 2_575 ?
O3 K1 U2 37.67(14) 1_565 . ?
O3 K1 U2 152.90(17) 1_565 4_465 ?
O3 K1 U2 39.01(14) 1_565 3 ?
O3 K1 O1 106.5(3) 2_565 1_565 ?
O3 K1 O1 106.5(3) 1_565 5_566 ?
O3 K1 O1 61.9(3) 2_565 5_566 ?
O3 K1 O1 61.9(3) 1_565 1_565 ?
O3 K1 O3 164.8(3) 1_565 2_565 ?
O3 K1 O5 66.9(2) 2_565 2_575 ?
O3 K1 O5 66.9(2) 1_565 . ?
O3 K1 O5 114.8(2) 1_565 2_575 ?
O3 K1 O5 114.8(2) 2_565 . ?
O3 K1 O6 66.1(2) 1_565 3 ?
O3 K1 O6 125.2(2) 2_565 3 ?
O3 K1 O6 125.2(2) 1_565 4_465 ?
O3 K1 O6 66.1(2) 2_565 4_465 ?
O5 K1 U2 150.28(14) . 2_575 ?
O5 K1 U2 150.28(15) 2_575 . ?
O5 K1 U2 89.91(15) 2_575 3 ?
O5 K1 U2 29.29(14) 2_575 2_575 ?
O5 K1 U2 84.89(15) . 3 ?
O5 K1 U2 29.29(14) . . ?
O5 K1 U2 84.89(15) 2_575 4_465 ?
O5 K1 U2 89.91(15) . 4_465 ?
O5 K1 O1 72.1(3) . 5_566 ?
O5 K1 O1 117.2(3) 2_575 5_566 ?
O5 K1 O1 117.2(3) . 1_565 ?
O5 K1 O1 72.1(3) 2_575 1_565 ?
O5 K1 O5 167.8(3) . 2_575 ?
O6 K1 U2 109.30(18) 3 4_465 ?
O6 K1 U2 92.28(16) 3 2_575 ?
O6 K1 U2 86.41(16) 4_465 2_575 ?
O6 K1 U2 27.69(15) 4_465 4_465 ?
O6 K1 U2 109.30(18) 4_465 3 ?
O6 K1 U2 86.41(16) 3 . ?
O6 K1 U2 27.69(15) 3 3 ?
O6 K1 U2 92.28(16) 4_465 . ?
O6 K1 O1 172.6(3) 4_465 1_565 ?
O6 K1 O1 85.9(2) 4_465 5_566 ?
O6 K1 O1 172.6(3) 3 5_566 ?
O6 K1 O1 85.9(2) 3 1_565 ?
O6 K1 O5 104.5(2) 3 . ?
O6 K1 O5 104.5(2) 4_465 2_575 ?
O6 K1 O5 67.1(2) 4_465 . ?
O6 K1 O5 67.1(2) 3 2_575 ?
O6 K1 O6 99.0(3) 4_465 3 ?
U1 O1 Cd2 132.4(5) . 5_566 ?
U1 O1 Cd2 132.4(5) . . ?
U1 O1 K1 104.4(3) . 5_566 ?
U1 O1 K1 104.4(3) . 1_545 ?
Cd2 O1 Cd2 15.19(16) . 5_566 ?
Cd2 O1 K1 114.0(4) 5_566 1_545 ?
Cd2 O1 K1 114.0(4) . 5_566 ?
Cd2 O1 K1 102.7(3) . 1_545 ?
Cd2 O1 K1 102.7(3) 5_566 5_566 ?
K1 O1 K1 90.1(3) 1_545 5_566 ?
U1 O2 Cd1 128.9(2) . 5_666 ?
U1 O2 Cd1 128.9(2) . 1_545 ?
Cd1 O2 Cd1 97.6(4) 5_666 1_545 ?
U1 O3 U2 107.5(3) . 3_545 ?
U1 O3 U2 136.0(3) . 1_545 ?
U1 O3 K1 104.2(3) . 1_545 ?
U2 O3 U2 109.5(3) 1_545 3_545 ?
U2 O3 K1 95.6(2) 1_545 1_545 ?
U2 O3 K1 94.9(2) 3_545 1_545 ?
U1 O4 U2 134.0(3) . . ?
U1 O4 U2 109.6(3) . 3_545 ?
U2 O4 U2 111.6(3) . 3_545 ?
U2 O5 Cd1 132.0(3) . 3_545 ?
U2 O5 Cd2 114.6(3) . . ?
U2 O5 K1 103.4(3) . . ?
Cd1 O5 Cd2 102.3(3) 3_545 . ?
Cd1 O5 K1 103.9(2) 3_545 . ?
Cd2 O5 K1 93.4(2) . . ?
U2 O6 Cd1 136.3(4) . . ?
U2 O6 K1 108.4(3) . 3_545 ?
Cd1 O6 K1 104.0(2) . 3_545 ?
U2 O7 U2 158.0(5) 6_556 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 U2 O5 Cd1 25.1(4) 3 . . 3_545 ?
U1 U2 O5 Cd2 161.8(3) 3 . . . ?
U1 U2 O5 K1 -98.1(2) 3 . . . ?
U1 U2 O6 Cd1 91.7(4) 3 . . . ?
U1 U2 O6 K1 -43.9(2) 3 . . 3_545 ?
U2 U2 O5 Cd1 89.5(4) 3 . . 3_545 ?
U2 U2 O5 Cd2 -133.8(2) 3 . . . ?
U2 U2 O5 K1 -33.7(2) 3 . . . ?
U2 U2 O6 Cd1 27.1(4) 3 . . . ?
U2 U2 O6 K1 -108.5(2) 3 . . 3_545 ?
Cd2 U2 O5 Cd1 -136.7(6) . . . 3_545 ?
Cd2 U2 O5 K1 100.1(4) . . . . ?
Cd2 U2 O6 Cd1 -107.1(5) . . . . ?
Cd2 U2 O6 K1 117.3(3) . . . 3_545 ?
K1 U2 O5 Cd1 -17.7(6) 3_545 . . 3_545 ?
K1 U2 O5 Cd1 123.2(5) . . . 3_545 ?
K1 U2 O5 Cd2 -100.1(4) . . . . ?
K1 U2 O5 Cd2 119.0(2) 3_545 . . . ?
K1 U2 O5 K1 -140.87(14) 3_545 . . . ?
K1 U2 O6 Cd1 -4.9(6) . . . . ?
K1 U2 O6 Cd1 135.6(6) 3_545 . . . ?
K1 U2 O6 K1 -140.55(15) . . . 3_545 ?
O3 U2 O5 Cd1 -8.4(4) 3 . . 3_545 ?
O3 U2 O5 Cd1 125.5(4) 1_565 . . 3_545 ?
O3 U2 O5 Cd2 128.3(3) 3 . . . ?
O3 U2 O5 Cd2 -97.8(3) 1_565 . . . ?
O3 U2 O5 K1 -131.6(3) 3 . . . ?
O3 U2 O5 K1 2.3(3) 1_565 . . . ?
O3 U2 O6 Cd1 125.3(5) 3 . . . ?
O3 U2 O6 Cd1 -8.7(4) 1_565 . . . ?
O3 U2 O6 K1 -10.4(3) 3 . . 3_545 ?
O3 U2 O6 K1 -144.4(3) 1_565 . . 3_545 ?
O4 U2 O5 Cd1 -75.4(5) . . . 3_545 ?
O4 U2 O5 Cd1 58.3(4) 3 . . 3_545 ?
O4 U2 O5 Cd2 61.3(3) . . . . ?
O4 U2 O5 Cd2 -165.0(3) 3 . . . ?
O4 U2 O5 K1 -64.9(3) 3 . . . ?
O4 U2 O5 K1 161.4(3) . . . . ?
O4 U2 O6 Cd1 58.6(5) 3 . . . ?
O4 U2 O6 Cd1 -167.8(5) . . . . ?
O4 U2 O6 K1 -77.0(3) 3 . . 3_545 ?
O4 U2 O6 K1 56.6(3) . . . 3_545 ?
O7 U2 O5 Cd1 -153.8(5) . . . 3_545 ?
O7 U2 O5 Cd2 -17.2(4) . . . . ?
O7 U2 O5 K1 83.0(3) . . . . ?
O7 U2 O6 Cd1 -89.3(5) . . . . ?
O7 U2 O6 K1 135.1(3) . . . 3_545 ?

_olex2_submission_special_instructions 'No special instructions were received'
# start Validation Reply Form
_vrf_PLAT196_pnnm_a              
;
PROBLEM: No TEMP record and _measurement_temperature .NE.        293 Degree
RESPONSE: The alert arises due to the low temperature (100 k) measurement.
;
_vrf_PLAT306_pnnm_a              
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) .......         O8 Check 
RESPONSE: No reliable hydrogen atoms can be added as O8 is disordered in partial 
occupancies.
;
_vrf_PLAT972_pnnm_a              
;
PROBLEM: Check Calcd Resid. Dens.  0.47Ang From K1             -3.33 eA-3  
RESPONSE: The alert arises due to strong absorption of uranium compounds.
;
# end Validation Reply Form
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_c2byc_a
_database_code_depnum_ccdc_archive 'CCDC 2244534'
loop_
_audit_author_name
_audit_author_address
'Yingjie Zhang'
;Australian Nuclear Science and Technology Organisation
Australia
;
_audit_update_record             
;
2023-02-25 deposited with the CCDC.	2023-04-25 downloaded from the CCDC.
;
_audit_creation_date             2022-12-16
_audit_creation_method           
;
Olex2 1.5
(compiled 2021.12.09 svn.r5202d8cf for OlexSys, GUI svn.r6439)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cd0.5 K2.5 O39 U11'
_chemical_formula_sum            'Cd0.50 K2.50 O39 U11'
_chemical_formula_weight         3396.28
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        C2/c
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   11.589(2)
_cell_length_b                   21.125(4)
_cell_length_c                   14.596(3)
_cell_angle_alpha                90
_cell_angle_beta                 104.23(3)
_cell_angle_gamma                90
_cell_volume                     3463.8(13)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    16000
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      24.996
_cell_measurement_theta_min      1.928
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    51.941
_exptl_absorpt_correction_T_max  0.4344
_exptl_absorpt_correction_T_min  0.3701
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2012/1 (Bruker,2012) was used for absorption correction.
wR2(int) was 0.2137 before and 0.0857 after correction.
The Ratio of minimum to maximum transmission is 0.8520.
The λ/2 correction factor is 0.0015.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    6.513
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       needle
_exptl_crystal_F_000             5582
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.010
_exptl_crystal_size_min          0.004
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.1056
_diffrn_reflns_av_unetI/netI     0.0643
_diffrn_reflns_Laue_measured_fraction_full 0.981
_diffrn_reflns_Laue_measured_fraction_max 0.981
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            19668
_diffrn_reflns_point_group_measured_fraction_full 0.981
_diffrn_reflns_point_group_measured_fraction_max 0.981
_diffrn_reflns_theta_full        24.996
_diffrn_reflns_theta_max         24.996
_diffrn_reflns_theta_min         1.928
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.981
_diffrn_radiation_type           
'silicon double crystal monochromated synchrotron'
_diffrn_source                   'Australian Synchrotron MX2'
_diffrn_measurement_device_type  'Eiger Detector'
_diffrn_measurement_method       'π  scans'
_diffrn_radiation_wavelength     0.71086
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                2426
_reflns_number_total             3001
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_data_collection       'BlueIce (McPhillips, et al., 2002)'
_computing_data_reduction        'XDS (Kabsch, 1993)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         11.137
_refine_diff_density_min         -2.932
_refine_diff_density_rms         0.895
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.114
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     204
_refine_ls_number_reflns         3001
_refine_ls_number_restraints     347
_refine_ls_R_factor_all          0.0634
_refine_ls_R_factor_gt           0.0538
_refine_ls_restrained_S_all      1.053
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0641P)²+242.9001P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1327
_refine_ls_wR_factor_ref         0.1488
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O2) = Uanis(O3) = Uanis(O4) = Uanis(O7) = Uanis(O8) = Uanis(O10) =
Uanis(O12) = Uanis(O14) = Uanis(O15)
2. Rigid body (RIGU) restrains
 All non-hydrogen atoms
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
3. Others
 Fixed Sof: Cd1(0.25) K2(0.375) K3(0.375) O6(0.5)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.750000 0.750000 0.500000 0.0170(3) Uani 1 2 d S . P . .
U2 U 0.44583(7) 0.75079(3) 0.50410(5) 0.0125(2) Uani 1 1 d . . . . .
U3 U 0.25394(6) 0.58899(3) 0.51802(5) 0.0093(2) Uani 1 1 d . . . . .
U4 U -0.06004(7) 0.57993(3) 0.51772(5) 0.0076(2) Uani 1 1 d . . . . .
U5 U -0.17937(7) 0.57483(3) 0.72669(6) 0.0120(2) Uani 1 1 d . . . . .
U6 U -0.42786(7) 0.57984(3) 0.52290(5) 0.0081(2) Uani 1 1 d . . . . .
Cd1 Cd 1.000000 0.82046(19) 0.750000 0.0133(8) Uani 0.5 2 d S T P . .
K1 K 0.000000 0.6161(4) 0.250000 0.0280(16) Uani 1 2 d S T P . .
K2 K -0.500000 0.4889(4) 0.750000 0.0164(17) Uani 0.75 2 d S T P . .
K3 K 0.500000 0.6641(5) 0.750000 0.039(3) Uani 0.75 2 d S T P . .
O1 O 0.8268(16) 0.7776(8) 0.6533(13) 0.037(4) Uani 1 1 d . . . . .
O2 O 0.6313(13) 0.6909(6) 0.5334(10) 0.0185(11) Uani 1 1 d . . . . .
O3 O 0.6172(13) 0.8113(6) 0.4842(10) 0.0185(11) Uani 1 1 d . . . . .
O4 O 0.4803(13) 0.7701(6) 0.6260(10) 0.0185(11) Uani 1 1 d . . . . .
O5 O 0.4138(15) 0.7284(7) 0.3810(11) 0.029(3) Uani 1 1 d . . . . .
O6 O 0.258(3) 0.7538(15) 0.5319(19) 0.023(6) Uani 0.5 1 d . . P . .
O7 O 0.4179(13) 0.6465(6) 0.5450(11) 0.0185(11) Uani 1 1 d . . . . .
O8 O 0.2830(14) 0.5710(6) 0.6515(11) 0.0185(11) Uani 1 1 d . . . . .
O9 O 0.2244(13) 0.6113(8) 0.3945(10) 0.023(3) Uani 1 1 d . . . . .
O10 O 0.1006(13) 0.5243(6) 0.4936(11) 0.0185(11) Uani 1 1 d . . . . .
O11 O 0.1008(13) 0.6451(7) 0.5323(11) 0.019(3) Uani 1 1 d . . . . .
O12 O -0.0062(14) 0.5745(6) 0.6551(11) 0.0185(11) Uani 1 1 d . . . . .
O13 O -0.1203(14) 0.5861(6) 0.3896(11) 0.015(3) Uani 1 1 d . . . . .
O14 O -0.2288(14) 0.5786(6) 0.5629(11) 0.0185(11) Uani 1 1 d . . . . .
O15 O -0.1683(13) 0.4908(7) 0.7256(11) 0.0185(11) Uani 1 1 d . . . . .
O16 O -0.1838(12) 0.6588(6) 0.7314(10) 0.015(3) Uani 1 1 d . . . . .
O17 O -0.4530(13) 0.5937(6) 0.3980(10) 0.015(3) Uani 1 1 d . . . . .
O18 O -0.3925(12) 0.5692(6) 0.6549(11) 0.016(3) Uani 1 1 d . . . . .
O19 O -0.3973(12) 0.4764(6) 0.4941(10) 0.015(3) Uani 1 1 d . . . . .
O20 O 1.1563(13) 0.8932(8) 0.7503(10) 0.025(4) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 U2 3.5402(10) . ?
U1 U2 3.5402(10) 7_666 ?
U1 O1 2.271(19) 7_666 ?
U1 O1 2.271(19) . ?
U1 O2 2.005(14) . ?
U1 O2 2.005(14) 7_666 ?
U1 O3 1.982(14) . ?
U1 O3 1.982(14) 7_666 ?
U2 U4 3.8535(12) 7_566 ?
U2 U6 3.8811(12) 1_655 ?
U2 K3 3.940(5) . ?
U2 O2 2.439(14) . ?
U2 O3 2.439(15) . ?
U2 O4 1.773(15) . ?
U2 O5 1.805(16) . ?
U2 O6 2.29(3) 7_566 ?
U2 O6 2.31(3) . ?
U2 O7 2.326(14) . ?
U2 O11 2.296(14) 7_566 ?
U3 U4 3.6427(12) . ?
U3 U5 4.0378(13) 2_556 ?
U3 U6 3.6758(12) 1_655 ?
U3 K1 4.3165(19) . ?
U3 K3 4.167(4) . ?
U3 O7 2.208(14) . ?
U3 O8 1.932(16) . ?
U3 O9 1.813(14) . ?
U3 O10 2.200(14) . ?
U3 O11 2.186(14) . ?
U3 O19 2.200(13) 5_566 ?
U4 U4 3.7367(15) 5_566 ?
U4 U5 4.0667(18) 2_556 ?
U4 U5 3.6472(13) . ?
U4 O3 2.389(13) 7_566 ?
U4 O10 2.301(14) . ?
U4 O10 2.249(14) 5_566 ?
U4 O11 2.284(14) . ?
U4 O12 1.951(16) . ?
U4 O13 1.833(15) . ?
U4 O14 2.213(16) . ?
U5 U5 4.0443(17) 2_556 ?
U5 U6 3.5973(17) . ?
U5 O8 2.379(16) 2_556 ?
U5 O12 2.404(16) 2_556 ?
U5 O12 2.480(16) . ?
U5 O14 2.319(16) . ?
U5 O15 1.781(14) . ?
U5 O16 1.777(14) . ?
U5 O18 2.437(14) . ?
U6 U6 3.7513(15) 5_466 ?
U6 K3 4.027(5) 1_455 ?
U6 O2 2.438(14) 1_455 ?
U6 O7 2.359(14) 1_455 ?
U6 O14 2.236(16) . ?
U6 O17 1.798(14) . ?
U6 O18 1.883(15) . ?
U6 O19 2.309(13) 5_466 ?
U6 O19 2.270(13) . ?
Cd1 K2 3.557(9) 3_655 ?
Cd1 O1 2.335(19) . ?
Cd1 O1 2.335(18) 2_756 ?
Cd1 O5 2.581(17) 8_566 ?
Cd1 O5 2.581(17) 7_666 ?
Cd1 O20 2.374(16) 2_756 ?
Cd1 O20 2.374(17) . ?
K1 O4 2.984(16) 8_465 ?
K1 O4 2.984(16) 7_566 ?
K1 O9 2.919(15) . ?
K1 O9 2.919(15) 2 ?
K1 O13 2.809(15) 2 ?
K1 O13 2.809(15) . ?
K1 O15 2.947(15) 5_566 ?
K1 O15 2.947(15) 6_565 ?
K2 K3 3.701(14) 1_455 ?
K2 O8 3.102(15) 1_455 ?
K2 O8 3.102(15) 2_556 ?
K2 O17 2.726(15) 6_566 ?
K2 O17 2.726(15) 5_466 ?
K2 O18 2.685(16) . ?
K2 O18 2.685(16) 2_456 ?
K2 O20 2.714(16) 4_546 ?
K2 O20 2.714(16) 3_345 ?
K3 O4 2.852(17) 2_656 ?
K3 O4 2.852(17) . ?
K3 O7 2.931(15) 2_656 ?
K3 O7 2.931(15) . ?
K3 O8 3.238(16) . ?
K3 O8 3.238(16) 2_656 ?
K3 O18 2.888(16) 1_655 ?
K3 O18 2.888(16) 2_556 ?
O6 O6 0.92(5) 7_566 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
U2 U1 U2 180.0 7_666 . ?
O1 U1 U2 82.4(5) 7_666 . ?
O1 U1 U2 97.6(5) 7_666 7_666 ?
O1 U1 U2 97.6(5) . . ?
O1 U1 U2 82.4(5) . 7_666 ?
O1 U1 O1 180.0 7_666 . ?
O2 U1 U2 41.7(4) . . ?
O2 U1 U2 41.7(4) 7_666 7_666 ?
O2 U1 U2 138.3(4) . 7_666 ?
O2 U1 U2 138.3(4) 7_666 . ?
O2 U1 O1 87.3(6) 7_666 . ?
O2 U1 O1 92.7(6) 7_666 7_666 ?
O2 U1 O1 87.3(6) . 7_666 ?
O2 U1 O1 92.7(6) . . ?
O2 U1 O2 180.0 . 7_666 ?
O3 U1 U2 41.5(4) 7_666 7_666 ?
O3 U1 U2 138.5(4) 7_666 . ?
O3 U1 U2 41.5(4) . . ?
O3 U1 U2 138.5(4) . 7_666 ?
O3 U1 O1 87.0(6) 7_666 . ?
O3 U1 O1 93.0(6) 7_666 7_666 ?
O3 U1 O1 87.0(6) . 7_666 ?
O3 U1 O1 93.0(6) . . ?
O3 U1 O2 82.9(6) . . ?
O3 U1 O2 97.1(6) 7_666 . ?
O3 U1 O2 82.9(6) 7_666 7_666 ?
O3 U1 O2 97.1(6) . 7_666 ?
O3 U1 O3 180.0(8) 7_666 . ?
U1 U2 U4 68.858(19) . 7_566 ?
U1 U2 U6 68.716(19) . 1_655 ?
U1 U2 K3 94.41(3) . . ?
U4 U2 U6 137.57(3) 7_566 1_655 ?
U4 U2 K3 121.72(13) 7_566 . ?
U6 U2 K3 61.97(13) 1_655 . ?
O2 U2 U1 33.1(3) . . ?
O2 U2 U4 101.0(3) . 7_566 ?
O2 U2 U6 37.3(3) . 1_655 ?
O2 U2 K3 70.3(3) . . ?
O3 U2 U1 32.6(3) . . ?
O3 U2 U4 36.6(3) . 7_566 ?
O3 U2 U6 101.1(3) . 1_655 ?
O3 U2 K3 113.6(4) . . ?
O3 U2 O2 65.5(5) . . ?
O4 U2 U1 92.2(5) . . ?
O4 U2 U4 82.7(5) . 7_566 ?
O4 U2 U6 98.9(4) . 1_655 ?
O4 U2 K3 41.1(5) . . ?
O4 U2 O2 88.4(6) . . ?
O4 U2 O3 90.6(6) . . ?
O4 U2 O5 177.9(7) . . ?
O4 U2 O6 101.8(9) . 7_566 ?
O4 U2 O6 78.8(8) . . ?
O4 U2 O7 88.3(6) . . ?
O4 U2 O11 89.7(6) . 7_566 ?
O5 U2 U1 86.8(6) . . ?
O5 U2 U4 98.7(5) . 7_566 ?
O5 U2 U6 79.0(5) . 1_655 ?
O5 U2 K3 137.1(5) . . ?
O5 U2 O2 89.8(6) . . ?
O5 U2 O3 89.6(6) . . ?
O5 U2 O6 79.2(9) . 7_566 ?
O5 U2 O6 102.1(9) . . ?
O5 U2 O7 90.0(6) . . ?
O5 U2 O11 92.4(6) . 7_566 ?
O6 U2 U1 165.9(7) 7_566 . ?
O6 U2 U1 171.0(7) . . ?
O6 U2 U4 110.3(8) . 7_566 ?
O6 U2 U4 112.1(8) 7_566 7_566 ?
O6 U2 U6 109.0(8) 7_566 1_655 ?
O6 U2 U6 111.6(8) . 1_655 ?
O6 U2 K3 78.4(7) . . ?
O6 U2 K3 96.5(7) 7_566 . ?
O6 U2 O2 144.2(9) . . ?
O6 U2 O2 146.3(9) 7_566 . ?
O6 U2 O3 144.9(9) 7_566 . ?
O6 U2 O3 146.7(8) . . ?
O6 U2 O6 23.0(13) 7_566 . ?
O6 U2 O7 77.6(9) . . ?
O6 U2 O7 79.5(9) 7_566 . ?
O6 U2 O11 79.5(9) 7_566 7_566 ?
O7 U2 U1 101.6(4) . . ?
O7 U2 U4 166.5(4) . 7_566 ?
O7 U2 U6 34.3(4) . 1_655 ?
O7 U2 K3 47.7(4) . . ?
O7 U2 O2 68.6(5) . . ?
O7 U2 O3 134.1(5) . . ?
O11 U2 U1 100.3(3) 7_566 . ?
O11 U2 U4 32.6(4) 7_566 7_566 ?
O11 U2 U6 166.2(3) 7_566 1_655 ?
O11 U2 K3 129.2(4) 7_566 . ?
O11 U2 O2 133.2(5) 7_566 . ?
O11 U2 O3 67.8(5) 7_566 . ?
O11 U2 O6 80.6(9) 7_566 . ?
O11 U2 O7 158.0(5) 7_566 . ?
U2 U3 K1 64.52(9) 7_566 . ?
U2 U3 K3 90.58(13) 7_566 . ?
U4 U3 U2 59.658(19) . 7_566 ?
U4 U3 U5 63.70(3) . 2_556 ?
U4 U3 U6 173.89(3) . 1_655 ?
U4 U3 K1 63.10(3) . . ?
U4 U3 K3 120.32(4) . . ?
U5 U3 U2 83.58(3) 2_556 7_566 ?
U5 U3 K1 126.39(2) 2_556 . ?
U5 U3 K3 62.44(5) 2_556 . ?
U6 U3 U2 126.43(3) 1_655 7_566 ?
U6 U3 U5 114.80(4) 1_655 2_556 ?
U6 U3 K1 118.80(3) 1_655 . ?
U6 U3 K3 61.41(5) 1_655 . ?
K3 U3 K1 149.75(17) . . ?
O7 U3 U2 90.3(3) . 7_566 ?
O7 U3 U4 147.7(4) . . ?
O7 U3 U5 104.2(4) . 2_556 ?
O7 U3 U6 37.8(4) . 1_655 ?
O7 U3 K1 117.0(4) . . ?
O7 U3 K3 42.1(4) . . ?
O8 U3 U2 101.5(4) . 7_566 ?
O8 U3 U4 85.2(5) . . ?
O8 U3 U5 22.8(4) . 2_556 ?
O8 U3 U6 92.6(5) . 1_655 ?
O8 U3 K1 148.3(5) . . ?
O8 U3 K3 48.8(4) . . ?
O8 U3 O7 90.0(6) . . ?
O8 U3 O10 88.5(6) . . ?
O8 U3 O11 87.4(6) . . ?
O8 U3 O19 90.6(6) . 5_566 ?
O9 U3 U2 74.9(5) . 7_566 ?
O9 U3 U4 93.9(5) . . ?
O9 U3 U5 155.0(5) . 2_556 ?
O9 U3 U6 88.6(5) . 1_655 ?
O9 U3 K1 31.1(5) . . ?
O9 U3 K3 129.3(5) . . ?
O9 U3 O7 88.8(6) . . ?
O9 U3 O8 176.2(7) . . ?
O9 U3 O10 93.0(6) . . ?
O9 U3 O11 89.7(6) . . ?
O9 U3 O19 92.6(6) . 5_566 ?
O10 U3 U2 94.7(4) . 7_566 ?
O10 U3 U4 36.9(4) . . ?
O10 U3 U5 75.9(4) . 2_556 ?
O10 U3 U6 137.5(4) . 1_655 ?
O10 U3 K1 65.9(4) . . ?
O10 U3 K3 137.1(4) . . ?
O10 U3 O7 175.0(5) . . ?
O11 U3 U2 25.5(4) . 7_566 ?
O11 U3 U4 36.3(4) . . ?
O11 U3 U5 65.8(4) . 2_556 ?
O11 U3 U6 149.4(4) . 1_655 ?
O11 U3 K1 68.0(4) . . ?
O11 U3 K3 97.2(4) . . ?
O11 U3 O7 111.6(5) . . ?
O11 U3 O10 73.1(5) . . ?
O11 U3 O19 173.9(5) . 5_566 ?
O19 U3 U2 160.3(3) 5_566 7_566 ?
O19 U3 U4 137.8(3) 5_566 . ?
O19 U3 U5 111.4(4) 5_566 2_556 ?
O19 U3 U6 36.4(3) 5_566 1_655 ?
O19 U3 K1 111.7(4) 5_566 . ?
O19 U3 K3 85.7(4) 5_566 . ?
O19 U3 O7 74.1(5) 5_566 . ?
O19 U3 O10 101.1(5) 5_566 . ?
U2 U4 U5 85.97(2) 7_566 2_556 ?
U3 U4 U2 65.67(2) . 7_566 ?
U3 U4 U4 69.01(3) . 5_566 ?
U3 U4 U5 125.77(4) . . ?
U3 U4 U5 62.89(3) . 2_556 ?
U4 U4 U2 132.85(4) 5_566 7_566 ?
U4 U4 U5 84.82(3) 5_566 2_556 ?
U5 U4 U2 107.76(2) . 7_566 ?
U5 U4 U4 108.65(3) . 5_566 ?
U5 U4 U5 62.97(3) . 2_556 ?
O3 U4 U2 37.5(3) 7_566 7_566 ?
O3 U4 U3 102.9(4) 7_566 . ?
O3 U4 U4 168.2(4) 7_566 5_566 ?
O3 U4 U5 99.3(4) 7_566 2_556 ?
O3 U4 U5 82.9(4) 7_566 . ?
O10 U4 U2 98.9(3) . 7_566 ?
O10 U4 U2 166.5(4) 5_566 7_566 ?
O10 U4 U3 35.1(3) . . ?
O10 U4 U3 104.0(4) 5_566 . ?
O10 U4 U4 34.3(3) . 5_566 ?
O10 U4 U4 35.2(4) 5_566 5_566 ?
O10 U4 U5 126.9(4) . . ?
O10 U4 U5 85.2(4) 5_566 . ?
O10 U4 U5 74.4(4) . 2_556 ?
O10 U4 U5 97.1(4) 5_566 2_556 ?
O10 U4 O3 152.6(5) 5_566 7_566 ?
O10 U4 O3 136.2(5) . 7_566 ?
O10 U4 O10 69.6(6) 5_566 . ?
O10 U4 O11 138.4(5) 5_566 . ?
O11 U4 U2 32.8(4) . 7_566 ?
O11 U4 U3 34.5(3) . . ?
O11 U4 U4 103.5(3) . 5_566 ?
O11 U4 U5 64.8(4) . 2_556 ?
O11 U4 U5 114.1(4) . . ?
O11 U4 O3 68.9(5) . 7_566 ?
O11 U4 O10 69.5(5) . . ?
O12 U4 U2 96.3(4) . 7_566 ?
O12 U4 U3 86.3(5) . . ?
O12 U4 U4 93.1(4) . 5_566 ?
O12 U4 U5 39.6(5) . . ?
O12 U4 U5 23.4(5) . 2_556 ?
O12 U4 O3 94.9(5) . 7_566 ?
O12 U4 O10 93.5(6) . . ?
O12 U4 O10 91.5(5) . 5_566 ?
O12 U4 O11 83.8(6) . . ?
O12 U4 O14 77.0(6) . . ?
O13 U4 U2 84.4(4) . 7_566 ?
O13 U4 U3 97.3(5) . . ?
O13 U4 U4 89.1(4) . 5_566 ?
O13 U4 U5 136.7(5) . . ?
O13 U4 U5 160.2(5) . 2_556 ?
O13 U4 O3 83.3(5) . 7_566 ?
O13 U4 O10 90.0(6) . . ?
O13 U4 O10 88.6(6) . 5_566 ?
O13 U4 O11 98.6(6) . . ?
O13 U4 O12 176.3(7) . . ?
O13 U4 O14 99.3(6) . . ?
O14 U4 U2 112.5(3) . 7_566 ?
O14 U4 U3 163.0(4) . . ?
O14 U4 U4 114.6(3) . 5_566 ?
O14 U4 U5 37.4(4) . . ?
O14 U4 U5 100.4(4) . 2_556 ?
O14 U4 O3 75.7(5) . 7_566 ?
O14 U4 O10 79.9(5) . 5_566 ?
O14 U4 O10 147.9(5) . . ?
O14 U4 O11 137.8(5) . . ?
U3 U5 U4 53.42(2) 2_556 2_556 ?
U3 U5 U5 106.80(4) 2_556 2_556 ?
U4 U5 U3 168.74(3) . 2_556 ?
U4 U5 U4 116.93(3) . 2_556 ?
U4 U5 U5 63.59(3) . 2_556 ?
U5 U5 U4 53.44(3) 2_556 2_556 ?
U6 U5 U3 116.84(3) . 2_556 ?
U6 U5 U4 169.97(3) . 2_556 ?
U6 U5 U4 72.46(3) . . ?
U6 U5 U5 136.05(4) . 2_556 ?
O8 U5 U3 18.4(4) 2_556 2_556 ?
O8 U5 U4 70.8(4) 2_556 2_556 ?
O8 U5 U4 172.3(4) 2_556 . ?
O8 U5 U5 124.1(4) 2_556 2_556 ?
O8 U5 U6 99.8(4) 2_556 . ?
O8 U5 O12 157.6(5) 2_556 . ?
O8 U5 O12 89.5(5) 2_556 2_556 ?
O8 U5 O18 71.0(5) 2_556 . ?
O12 U5 U3 140.2(4) . 2_556 ?
O12 U5 U3 72.2(4) 2_556 2_556 ?
O12 U5 U4 98.3(4) 2_556 . ?
O12 U5 U4 18.8(4) 2_556 2_556 ?
O12 U5 U4 86.9(4) . 2_556 ?
O12 U5 U4 30.1(4) . . ?
O12 U5 U5 33.5(4) . 2_556 ?
O12 U5 U5 34.7(4) 2_556 2_556 ?
O12 U5 U6 170.6(4) 2_556 . ?
O12 U5 U6 102.6(4) . . ?
O12 U5 O12 68.2(6) 2_556 . ?
O12 U5 O18 160.4(5) 2_556 . ?
O14 U5 U3 153.4(4) . 2_556 ?
O14 U5 U4 35.4(4) . . ?
O14 U5 U4 152.2(4) . 2_556 ?
O14 U5 U5 99.0(4) . 2_556 ?
O14 U5 U6 37.0(4) . . ?
O14 U5 O8 136.8(5) . 2_556 ?
O14 U5 O12 65.6(5) . . ?
O14 U5 O12 133.7(6) . 2_556 ?
O14 U5 O18 65.9(5) . . ?
O15 U5 U3 96.6(5) . 2_556 ?
O15 U5 U4 90.0(5) . 2_556 ?
O15 U5 U4 88.8(5) . . ?
O15 U5 U5 85.9(5) . 2_556 ?
O15 U5 U6 93.8(5) . . ?
O15 U5 O8 91.3(6) . 2_556 ?
O15 U5 O12 87.1(6) . 2_556 ?
O15 U5 O12 85.8(6) . . ?
O15 U5 O14 91.4(6) . . ?
O15 U5 O18 90.9(6) . . ?
O16 U5 U3 82.9(4) . 2_556 ?
O16 U5 U4 91.3(4) . . ?
O16 U5 U4 87.6(5) . 2_556 ?
O16 U5 U5 91.8(4) . 2_556 ?
O16 U5 U6 88.7(5) . . ?
O16 U5 O8 88.9(5) . 2_556 ?
O16 U5 O12 90.2(6) . 2_556 ?
O16 U5 O12 93.0(5) . . ?
O16 U5 O14 90.2(6) . . ?
O16 U5 O15 177.4(7) . . ?
O16 U5 O18 91.7(5) . . ?
O18 U5 U3 88.6(4) . 2_556 ?
O18 U5 U4 101.2(4) . . ?
O18 U5 U4 141.8(4) . 2_556 ?
O18 U5 U5 164.5(4) . 2_556 ?
O18 U5 U6 29.0(4) . . ?
O18 U5 O12 131.2(5) . . ?
U2 U6 K3 59.74(13) 1_455 1_455 ?
U3 U6 U2 65.83(2) 1_455 1_455 ?
U3 U6 U6 69.07(3) 1_455 5_466 ?
U3 U6 K3 65.32(4) 1_455 1_455 ?
U5 U6 U2 107.29(2) . 1_455 ?
U5 U6 U3 127.80(3) . 1_455 ?
U5 U6 U6 110.61(3) . 5_466 ?
U5 U6 K3 67.56(4) . 1_455 ?
U6 U6 U2 132.87(4) 5_466 1_455 ?
U6 U6 K3 111.74(13) 5_466 1_455 ?
O2 U6 U2 37.3(3) 1_455 1_455 ?
O2 U6 U3 102.5(3) 1_455 1_455 ?
O2 U6 U5 79.7(3) 1_455 . ?
O2 U6 U6 169.3(3) 1_455 5_466 ?
O2 U6 K3 68.6(4) 1_455 1_455 ?
O7 U6 U2 33.8(3) 1_455 1_455 ?
O7 U6 U3 35.0(3) 1_455 1_455 ?
O7 U6 U5 112.6(4) 1_455 . ?
O7 U6 U6 104.0(3) 1_455 5_466 ?
O7 U6 K3 46.0(4) 1_455 1_455 ?
O7 U6 O2 68.1(5) 1_455 1_455 ?
O14 U6 U2 112.1(3) . 1_455 ?
O14 U6 U3 166.2(4) . 1_455 ?
O14 U6 U5 38.6(4) . . ?
O14 U6 U6 115.0(3) . 5_466 ?
O14 U6 K3 101.5(4) . 1_455 ?
O14 U6 O2 74.9(5) . 1_455 ?
O14 U6 O7 137.6(5) . 1_455 ?
O14 U6 O19 147.5(5) . 5_466 ?
O14 U6 O19 80.7(5) . . ?
O17 U6 U2 79.2(4) . 1_455 ?
O17 U6 U3 93.4(5) . 1_455 ?
O17 U6 U5 137.8(5) . . ?
O17 U6 U6 90.7(4) . 5_466 ?
O17 U6 K3 138.4(4) . 1_455 ?
O17 U6 O2 83.1(6) . 1_455 ?
O17 U6 O7 95.8(6) . 1_455 ?
O17 U6 O14 99.6(6) . . ?
O17 U6 O18 176.0(6) . . ?
O17 U6 O19 93.2(6) . 5_466 ?
O17 U6 O19 87.9(6) . . ?
O18 U6 U2 99.6(4) . 1_455 ?
O18 U6 U3 89.5(4) . 1_455 ?
O18 U6 U5 38.9(4) . . ?
O18 U6 U6 92.9(4) . 5_466 ?
O18 U6 K3 41.1(4) . 1_455 ?
O18 U6 O2 93.6(5) . 1_455 ?
O18 U6 O7 85.0(6) . 1_455 ?
O18 U6 O14 77.3(6) . . ?
O18 U6 O19 94.0(5) . . ?
O18 U6 O19 90.8(6) . 5_466 ?
O19 U6 U2 163.0(4) . 1_455 ?
O19 U6 U2 99.5(3) 5_466 1_455 ?
O19 U6 U3 104.4(3) . 1_455 ?
O19 U6 U3 34.4(3) 5_466 1_455 ?
O19 U6 U5 125.2(4) 5_466 . ?
O19 U6 U5 89.7(4) . . ?
O19 U6 U6 35.3(3) . 5_466 ?
O19 U6 U6 34.7(3) 5_466 5_466 ?
O19 U6 K3 87.8(3) 5_466 1_455 ?
O19 U6 K3 130.6(4) . 1_455 ?
O19 U6 O2 152.1(5) . 1_455 ?
O19 U6 O2 136.6(5) 5_466 1_455 ?
O19 U6 O7 69.3(5) 5_466 1_455 ?
O19 U6 O7 139.3(5) . 1_455 ?
O19 U6 O19 70.0(5) . 5_466 ?
O1 Cd1 K2 112.8(4) 2_756 3_655 ?
O1 Cd1 K2 112.8(4) . 3_655 ?
O1 Cd1 O1 134.3(8) . 2_756 ?
O1 Cd1 O5 82.0(6) . 8_566 ?
O1 Cd1 O5 80.1(6) . 7_666 ?
O1 Cd1 O5 80.1(6) 2_756 8_566 ?
O1 Cd1 O5 82.0(6) 2_756 7_666 ?
O1 Cd1 O20 142.6(6) . . ?
O1 Cd1 O20 73.0(6) . 2_756 ?
O1 Cd1 O20 73.0(6) 2_756 . ?
O1 Cd1 O20 142.6(6) 2_756 2_756 ?
O5 Cd1 K2 113.6(3) 8_566 3_655 ?
O5 Cd1 K2 113.6(3) 7_666 3_655 ?
O5 Cd1 O5 132.8(7) 7_666 8_566 ?
O20 Cd1 K2 49.7(4) 2_756 3_655 ?
O20 Cd1 K2 49.7(4) . 3_655 ?
O20 Cd1 O5 133.8(5) 2_756 7_666 ?
O20 Cd1 O5 80.0(5) . 7_666 ?
O20 Cd1 O5 133.8(5) . 8_566 ?
O20 Cd1 O5 80.0(5) 2_756 8_566 ?
O20 Cd1 O20 99.4(8) . 2_756 ?
U3 K1 U3 164.8(2) 2 . ?
U4 K1 U3 50.60(2) 2 2 ?
U4 K1 U3 125.91(7) . 2 ?
U4 K1 U3 50.60(2) . . ?
U4 K1 U3 125.91(7) 2 . ?
U4 K1 U4 159.1(2) . 2 ?
O4 K1 U3 67.9(3) 7_566 . ?
O4 K1 U3 126.1(3) 7_566 2 ?
O4 K1 U3 126.1(3) 8_465 . ?
O4 K1 U3 67.9(3) 8_465 2 ?
O4 K1 U4 65.7(3) 7_566 . ?
O4 K1 U4 134.8(3) 8_465 . ?
O4 K1 U4 134.8(3) 7_566 2 ?
O4 K1 U4 65.7(3) 8_465 2 ?
O4 K1 O4 72.6(6) 7_566 8_465 ?
O9 K1 U3 18.7(3) 2 2 ?
O9 K1 U3 159.7(3) . 2 ?
O9 K1 U3 159.7(3) 2 . ?
O9 K1 U3 18.7(3) . . ?
O9 K1 U4 69.1(3) 2 2 ?
O9 K1 U4 110.1(3) . 2 ?
O9 K1 U4 69.1(3) . . ?
O9 K1 U4 110.1(3) 2 . ?
O9 K1 O4 112.8(4) . 8_465 ?
O9 K1 O4 70.6(4) . 7_566 ?
O9 K1 O4 112.8(4) 2 7_566 ?
O9 K1 O4 70.6(4) 2 8_465 ?
O9 K1 O9 176.0(7) . 2 ?
O9 K1 O15 56.0(4) . 5_566 ?
O9 K1 O15 56.0(4) 2 6_565 ?
O9 K1 O15 120.4(5) 2 5_566 ?
O9 K1 O15 120.4(5) . 6_565 ?
O13 K1 U3 70.3(3) . . ?
O13 K1 U3 106.1(3) . 2 ?
O13 K1 U3 106.1(3) 2 . ?
O13 K1 U3 70.3(3) 2 2 ?
O13 K1 U4 19.9(3) . . ?
O13 K1 U4 19.9(3) 2 2 ?
O13 K1 U4 149.1(3) . 2 ?
O13 K1 U4 149.1(3) 2 . ?
O13 K1 O4 130.0(4) . 8_465 ?
O13 K1 O4 73.7(4) 2 8_465 ?
O13 K1 O4 130.0(4) 2 7_566 ?
O13 K1 O4 73.7(4) . 7_566 ?
O13 K1 O9 88.9(4) . . ?
O13 K1 O9 90.2(4) 2 . ?
O13 K1 O9 88.9(4) 2 2 ?
O13 K1 O9 90.2(4) . 2 ?
O13 K1 O13 154.0(6) . 2 ?
O13 K1 O15 58.9(4) 2 5_566 ?
O13 K1 O15 58.9(4) . 6_565 ?
O13 K1 O15 99.9(4) 2 6_565 ?
O13 K1 O15 99.9(4) . 5_566 ?
O15 K1 U3 106.9(3) 6_565 . ?
O15 K1 U3 60.4(3) 6_565 2 ?
O15 K1 U3 106.9(3) 5_566 2 ?
O15 K1 U3 60.4(3) 5_566 . ?
O15 K1 U4 90.3(3) 5_566 . ?
O15 K1 U4 73.6(3) 5_566 2 ?
O15 K1 U4 90.3(3) 6_565 2 ?
O15 K1 U4 73.6(3) 6_565 . ?
O15 K1 O4 129.8(4) 6_565 7_566 ?
O15 K1 O4 126.5(4) 5_566 7_566 ?
O15 K1 O4 129.8(4) 5_566 8_465 ?
O15 K1 O4 126.5(4) 6_565 8_465 ?
O15 K1 O15 80.0(6) 6_565 5_566 ?
U6 K2 U6 124.0(2) 2_456 . ?
Cd1 K2 U6 118.02(10) 3_345 . ?
Cd1 K2 U6 118.02(10) 3_345 2_456 ?
Cd1 K2 K3 180.0 3_345 1_455 ?
K3 K2 U6 61.98(10) 1_455 . ?
K3 K2 U6 61.98(10) 1_455 2_456 ?
O8 K2 U6 70.5(3) 2_556 2_456 ?
O8 K2 U6 79.0(3) 1_455 2_456 ?
O8 K2 U6 70.5(3) 1_455 . ?
O8 K2 U6 79.0(3) 2_556 . ?
O8 K2 Cd1 124.0(3) 2_556 3_345 ?
O8 K2 Cd1 124.0(3) 1_455 3_345 ?
O8 K2 K3 56.0(3) 1_455 1_455 ?
O8 K2 K3 56.0(3) 2_556 1_455 ?
O8 K2 O8 112.0(6) 2_556 1_455 ?
O17 K2 U6 154.4(3) 6_566 . ?
O17 K2 U6 72.5(3) 6_566 2_456 ?
O17 K2 U6 154.4(3) 5_466 2_456 ?
O17 K2 U6 72.5(3) 5_466 . ?
O17 K2 Cd1 50.2(3) 5_466 3_345 ?
O17 K2 Cd1 50.2(3) 6_566 3_345 ?
O17 K2 K3 129.8(3) 6_566 1_455 ?
O17 K2 K3 129.8(3) 5_466 1_455 ?
O17 K2 O8 90.5(4) 5_466 1_455 ?
O17 K2 O8 90.5(4) 6_566 2_556 ?
O17 K2 O8 135.0(4) 5_466 2_556 ?
O17 K2 O8 135.0(4) 6_566 1_455 ?
O17 K2 O17 100.4(6) 5_466 6_566 ?
O18 K2 U6 21.8(3) . . ?
O18 K2 U6 109.6(4) 2_456 . ?
O18 K2 U6 21.8(3) 2_456 2_456 ?
O18 K2 U6 109.6(4) . 2_456 ?
O18 K2 Cd1 129.2(3) 2_456 3_345 ?
O18 K2 Cd1 129.2(3) . 3_345 ?
O18 K2 K3 50.8(3) . 1_455 ?
O18 K2 K3 50.8(3) 2_456 1_455 ?
O18 K2 O8 80.4(4) . 1_455 ?
O18 K2 O8 80.4(4) 2_456 2_556 ?
O18 K2 O8 57.3(5) . 2_556 ?
O18 K2 O8 57.3(5) 2_456 1_455 ?
O18 K2 O17 141.9(4) . 6_566 ?
O18 K2 O17 91.3(4) . 5_466 ?
O18 K2 O17 141.9(4) 2_456 5_466 ?
O18 K2 O17 91.3(4) 2_456 6_566 ?
O18 K2 O18 101.6(6) . 2_456 ?
O18 K2 O20 149.8(4) . 4_546 ?
O18 K2 O20 94.4(4) 2_456 4_546 ?
O18 K2 O20 94.4(4) . 3_345 ?
O18 K2 O20 149.8(4) 2_456 3_345 ?
O20 K2 U6 94.7(3) 4_546 2_456 ?
O20 K2 U6 128.2(3) 3_345 2_456 ?
O20 K2 U6 128.2(3) 4_546 . ?
O20 K2 U6 94.7(3) 3_345 . ?
O20 K2 Cd1 41.9(4) 4_546 3_345 ?
O20 K2 Cd1 41.9(4) 3_345 3_345 ?
O20 K2 K3 138.1(4) 4_546 1_455 ?
O20 K2 K3 138.1(4) 3_345 1_455 ?
O20 K2 O8 87.2(4) 4_546 1_455 ?
O20 K2 O8 151.9(4) 3_345 1_455 ?
O20 K2 O8 151.9(4) 4_546 2_556 ?
O20 K2 O8 87.2(4) 3_345 2_556 ?
O20 K2 O17 61.2(5) 3_345 6_566 ?
O20 K2 O17 61.2(5) 4_546 5_466 ?
O20 K2 O17 61.8(5) 4_546 6_566 ?
O20 K2 O17 61.8(5) 3_345 5_466 ?
O20 K2 O20 83.7(7) 4_546 3_345 ?
U2 K3 U2 124.6(3) . 2_656 ?
U2 K3 U6 58.295(19) . 1_655 ?
U2 K3 U6 159.47(3) 2_656 1_655 ?
K2 K3 U2 117.71(14) 1_655 2_656 ?
K2 K3 U2 117.71(14) 1_655 . ?
K2 K3 U6 63.78(14) 1_655 1_655 ?
O4 K3 U2 100.5(4) 2_656 . ?
O4 K3 U2 100.5(4) . 2_656 ?
O4 K3 U2 24.1(3) . . ?
O4 K3 U2 24.1(3) 2_656 2_656 ?
O4 K3 U6 79.9(3) . 1_655 ?
O4 K3 U6 150.3(4) 2_656 1_655 ?
O4 K3 K2 141.7(3) . 1_655 ?
O4 K3 K2 141.7(3) 2_656 1_655 ?
O4 K3 O4 76.6(6) 2_656 . ?
O4 K3 O7 59.8(4) 2_656 2_656 ?
O4 K3 O7 134.6(5) 2_656 . ?
O4 K3 O7 59.8(4) . . ?
O4 K3 O7 134.6(5) . 2_656 ?
O4 K3 O8 105.2(4) . . ?
O4 K3 O8 133.7(4) . 2_656 ?
O4 K3 O8 133.7(4) 2_656 . ?
O4 K3 O8 105.2(4) 2_656 2_656 ?
O4 K3 O18 102.5(4) 2_656 2_556 ?
O4 K3 O18 150.8(4) 2_656 1_655 ?
O4 K3 O18 150.8(4) . 2_556 ?
O4 K3 O18 102.5(4) . 1_655 ?
O7 K3 U2 158.1(4) 2_656 . ?
O7 K3 U2 158.1(4) . 2_656 ?
O7 K3 U2 35.9(3) . . ?
O7 K3 U2 35.9(3) 2_656 2_656 ?
O7 K3 U6 35.4(3) . 1_655 ?
O7 K3 U6 134.7(4) 2_656 1_655 ?
O7 K3 K2 82.7(3) 2_656 1_655 ?
O7 K3 K2 82.7(3) . 1_655 ?
O7 K3 O7 165.4(7) 2_656 . ?
O7 K3 O8 56.5(4) . . ?
O7 K3 O8 113.5(4) 2_656 . ?
O7 K3 O8 56.5(4) 2_656 2_656 ?
O7 K3 O8 113.5(4) . 2_656 ?
O8 K3 U2 128.3(3) 2_656 . ?
O8 K3 U2 86.9(3) . . ?
O8 K3 U2 128.3(3) . 2_656 ?
O8 K3 U2 86.9(3) 2_656 2_656 ?
O8 K3 U6 78.5(3) 2_656 1_655 ?
O8 K3 U6 70.2(3) . 1_655 ?
O8 K3 K2 52.6(3) 2_656 1_655 ?
O8 K3 K2 52.6(3) . 1_655 ?
O8 K3 O8 105.2(6) 2_656 . ?
O18 K3 U2 140.3(3) 1_655 2_656 ?
O18 K3 U2 82.9(3) 2_556 2_656 ?
O18 K3 U2 140.3(3) 2_556 . ?
O18 K3 U2 82.9(3) 1_655 . ?
O18 K3 U6 106.9(4) 2_556 1_655 ?
O18 K3 U6 25.4(3) 1_655 1_655 ?
O18 K3 K2 46.1(3) 2_556 1_655 ?
O18 K3 K2 46.1(3) 1_655 1_655 ?
O18 K3 O7 109.4(5) 1_655 2_656 ?
O18 K3 O7 109.4(5) 2_556 . ?
O18 K3 O7 59.5(4) 1_655 . ?
O18 K3 O7 59.5(4) 2_556 2_656 ?
O18 K3 O8 54.0(5) 1_655 2_656 ?
O18 K3 O8 54.0(5) 2_556 . ?
O18 K3 O8 75.2(4) 2_556 2_656 ?
O18 K3 O8 75.2(4) 1_655 . ?
O18 K3 O18 92.1(7) 1_655 2_556 ?
U1 O1 Cd1 140.0(8) . . ?
U1 O2 U2 105.2(6) . . ?
U1 O2 U6 141.5(7) . 1_655 ?
U6 O2 U2 105.4(5) 1_655 . ?
U1 O3 U2 106.0(6) . . ?
U1 O3 U4 146.6(7) . 7_566 ?
U4 O3 U2 105.9(5) 7_566 . ?
U2 O4 K1 139.3(7) . 7_566 ?
U2 O4 K3 114.8(6) . . ?
K3 O4 K1 105.4(5) . 7_566 ?
U2 O5 Cd1 145.0(9) . 7_666 ?
U2 O6 U2 157.0(13) 7_566 . ?
O6 O6 U2 77(4) 7_566 . ?
O6 O6 U2 80(4) 7_566 7_566 ?
U2 O7 U6 111.9(6) . 1_655 ?
U2 O7 K3 96.4(5) . . ?
U3 O7 U2 130.0(6) . . ?
U3 O7 U6 107.2(5) . 1_655 ?
U3 O7 K3 107.5(6) . . ?
U6 O7 K3 98.5(5) 1_655 . ?
U3 O8 U5 138.8(8) . 2_556 ?
U3 O8 K2 119.9(6) . 1_655 ?
U3 O8 K3 104.6(6) . . ?
U5 O8 K2 100.0(5) 2_556 1_655 ?
U5 O8 K3 97.3(5) 2_556 . ?
K2 O8 K3 71.4(4) 1_655 . ?
U3 O9 K1 130.1(7) . . ?
U3 O10 U4 140.0(7) . 5_566 ?
U3 O10 U4 108.0(6) . . ?
U4 O10 U4 110.4(6) 5_566 . ?
U3 O11 U2 130.4(6) . 7_566 ?
U3 O11 U4 109.1(6) . . ?
U4 O11 U2 114.5(6) . 7_566 ?
U4 O12 U5 137.8(8) . 2_556 ?
U4 O12 U5 110.2(7) . . ?
U5 O12 U5 111.8(6) 2_556 . ?
U4 O13 K1 128.6(7) . . ?
U4 O14 U5 107.2(6) . . ?
U4 O14 U6 148.5(8) . . ?
U6 O14 U5 104.3(6) . . ?
U5 O15 K1 144.1(7) . 5_566 ?
U6 O17 K2 130.5(7) . 5_466 ?
U5 O18 K2 111.0(6) . . ?
U5 O18 K3 105.7(5) . 1_455 ?
U6 O18 U5 112.1(7) . . ?
U6 O18 K2 126.3(6) . . ?
U6 O18 K3 113.5(6) . 1_455 ?
K2 O18 K3 83.1(5) . 1_455 ?
U3 O19 U6 109.2(6) 5_566 5_466 ?
U3 O19 U6 140.8(6) 5_566 . ?
U6 O19 U6 110.0(5) . 5_466 ?
Cd1 O20 K2 88.5(5) . 3_655 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
U1 U2 O4 K1 95.0(10) . . . 7_566 ?
U1 U2 O4 K3 -94.2(5) . . . . ?
U1 U2 O5 Cd1 20.2(13) . . . 7_666 ?
U2 U3 O9 K1 -65.4(8) 7_566 . . . ?
U2 U4 O13 K1 54.7(6) 7_566 . . . ?
U2 U6 O17 K2 -152.7(9) 1_455 . . 5_466 ?
U2 U6 O18 U5 -105.7(5) 1_455 . . . ?
U2 U6 O18 K2 113.1(7) 1_455 . . . ?
U2 U6 O18 K3 14.0(6) 1_455 . . 1_455 ?
U3 U4 O13 K1 -9.8(7) . . . . ?
U3 U5 O15 K1 -103.7(12) 2_556 . . 5_566 ?
U3 U6 O17 K2 -88.1(8) 1_455 . . 5_466 ?
U3 U6 O18 U5 -171.1(5) 1_455 . . . ?
U3 U6 O18 K2 47.7(7) 1_455 . . . ?
U3 U6 O18 K3 -51.4(5) 1_455 . . 1_455 ?
U4 U2 O4 K1 26.6(9) 7_566 . . 7_566 ?
U4 U2 O4 K3 -162.5(6) 7_566 . . . ?
U4 U2 O5 Cd1 88.3(13) 7_566 . . 7_666 ?
U4 U3 O9 K1 -8.3(9) . . . . ?
U4 U4 O13 K1 -78.5(7) 5_566 . . . ?
U4 U5 O15 K1 66.4(12) . . . 5_566 ?
U4 U5 O15 K1 -50.6(12) 2_556 . . 5_566 ?
U5 U3 O9 K1 -33.7(19) 2_556 . . . ?
U5 U4 O13 K1 -6.4(17) 2_556 . . . ?
U5 U4 O13 K1 164.7(3) . . . . ?
U5 U5 O15 K1 2.8(11) 2_556 . . 5_566 ?
U5 U6 O17 K2 103.4(8) . . . 5_466 ?
U5 U6 O18 K2 -141.2(11) . . . . ?
U5 U6 O18 K3 119.7(9) . . . 1_455 ?
U6 U2 O4 K1 163.8(9) 1_655 . . 7_566 ?
U6 U2 O4 K3 -25.4(6) 1_655 . . . ?
U6 U2 O5 Cd1 -48.7(12) 1_655 . . 7_666 ?
U6 U3 O9 K1 166.1(9) 1_655 . . . ?
U6 U5 O15 K1 138.7(12) . . . 5_566 ?
U6 U6 O17 K2 -19.1(8) 5_466 . . 5_466 ?
U6 U6 O18 U5 119.9(5) 5_466 . . . ?
U6 U6 O18 K2 -21.3(7) 5_466 . . . ?
U6 U6 O18 K3 -120.4(5) 5_466 . . 1_455 ?
K3 U2 O4 K1 -170.9(15) . . . 7_566 ?
K3 U2 O5 Cd1 -72.8(16) . . . 7_666 ?
K3 U3 O9 K1 -143.5(6) . . . . ?
K3 U6 O17 K2 -143.9(5) 1_455 . . 5_466 ?
K3 U6 O18 U5 -119.7(9) 1_455 . . . ?
K3 U6 O18 K2 99.1(9) 1_455 . . . ?
O2 U2 O4 K1 127.9(10) . . . 7_566 ?
O2 U2 O4 K3 -61.2(6) . . . . ?
O2 U2 O5 Cd1 -12.8(13) . . . 7_666 ?
O2 U6 O17 K2 169.7(9) 1_455 . . 5_466 ?
O2 U6 O18 U5 -68.6(6) 1_455 . . . ?
O2 U6 O18 K2 150.2(7) 1_455 . . . ?
O2 U6 O18 K3 51.1(6) 1_455 . . 1_455 ?
O3 U2 O4 K1 62.4(10) . . . 7_566 ?
O3 U2 O4 K3 -126.7(6) . . . . ?
O3 U2 O5 Cd1 52.7(13) . . . 7_666 ?
O3 U4 O13 K1 92.4(8) 7_566 . . . ?
O6 U2 O4 K1 -84.5(13) 7_566 . . 7_566 ?
O6 U2 O4 K1 -85.8(13) . . . 7_566 ?
O6 U2 O4 K3 85.1(10) . . . . ?
O6 U2 O4 K3 86.4(10) 7_566 . . . ?
O6 U2 O5 Cd1 -158.7(15) . . . 7_666 ?
O6 U2 O5 Cd1 -160.8(16) 7_566 . . 7_666 ?
O7 U2 O4 K1 -163.4(10) . . . 7_566 ?
O7 U2 O4 K3 7.4(6) . . . . ?
O7 U2 O5 Cd1 -81.4(14) . . . 7_666 ?
O7 U3 O9 K1 -156.0(10) . . . . ?
O7 U6 O17 K2 -123.2(8) 1_455 . . 5_466 ?
O7 U6 O18 U5 -136.3(6) 1_455 . . . ?
O7 U6 O18 K2 82.5(8) 1_455 . . . ?
O7 U6 O18 K3 -16.6(6) 1_455 . . 1_455 ?
O8 U5 O15 K1 -121.4(12) 2_556 . . 5_566 ?
O10 U3 O9 K1 28.7(10) . . . . ?
O10 U4 O13 K1 -113.8(8) 5_566 . . . ?
O10 U4 O13 K1 -44.2(8) . . . . ?
O11 U2 O4 K1 -5.4(10) 7_566 . . 7_566 ?
O11 U2 O4 K3 165.5(6) 7_566 . . . ?
O11 U2 O5 Cd1 120.5(13) 7_566 . . 7_666 ?
O11 U3 O9 K1 -44.4(10) . . . . ?
O11 U4 O13 K1 25.1(8) . . . . ?
O12 U5 O15 K1 36.3(12) . . . 5_566 ?
O12 U5 O15 K1 -32.0(12) 2_556 . . 5_566 ?
O14 U4 O13 K1 166.7(7) . . . . ?
O14 U5 O15 K1 101.7(12) . . . 5_566 ?
O14 U6 O17 K2 96.4(9) . . . 5_466 ?
O14 U6 O18 U5 5.0(5) . . . . ?
O14 U6 O18 K2 -136.2(8) . . . . ?
O14 U6 O18 K3 124.7(7) . . . 1_455 ?
O18 U5 O15 K1 167.6(12) . . . 5_566 ?
O19 U3 O9 K1 130.0(9) 5_566 . . . ?
O19 U6 O17 K2 16.2(9) . . . 5_466 ?
O19 U6 O17 K2 -53.7(9) 5_466 . . 5_466 ?
O19 U6 O18 U5 154.5(6) 5_466 . . . ?
O19 U6 O18 U5 84.5(6) . . . . ?
O19 U6 O18 K2 -56.7(8) . . . . ?
O19 U6 O18 K2 13.3(8) 5_466 . . . ?
O19 U6 O18 K3 -155.8(6) . . . 1_455 ?
O19 U6 O18 K3 -85.8(6) 5_466 . . 1_455 ?

_olex2_submission_special_instructions 'No special instructions were received'
# start Validation Reply Form
_vrf_PLAT971_c2byc_a             
;
PROBLEM: Check Calcd Resid. Dens.  0.24Ang From U3             10.05 eA-3  
RESPONSE: The strong Q-peaks around U atoms are common for U oxide compounds.
The alert arises due to the ineffective absorption corrections as only 
one-circle data collection is available on MX2 at the Australian Synchrotron.
;
_vrf_PLAT973_c2byc_a             
;
PROBLEM: Check Calcd Positive Resid. Density on        U1      10.95 eA-3  
RESPONSE: The strong Q-peaks around U atoms are common for U oxide compounds.
The alert arises due to the ineffective absorption corrections as only 
one-circle data collection is available on MX2 at the Australian Synchrotron.
;
_vrf_PLAT975_c2byc_a             
;
PROBLEM: Check Calcd Resid. Dens.  0.47Ang From O8      .       2.59 eA-3  
RESPONSE: The alert arises due to the strong absorptions for heavy U atoms.
;
_vrf_PLAT976_c2byc_a             
;
PROBLEM: Check Calcd Resid. Dens.  0.91Ang From O3      .      -2.21 eA-3  
RESPONSE: The alert arises due to the strong absorptions for heavy U atoms.
;
_vrf_PLAT097_c2byc_a             
;
PROBLEM: Large Reported Max.  (Positive) Residual Density      11.14 eA-3  
RESPONSE: The strong Q-peaks around U atoms are common for U oxide compounds.
The alert arises due to the ineffective absorption corrections as only 
one-circle data collection is available on MX2 at the Australian Synchrotron.
;
_vrf_PLAT196_c2byc_a             
;
PROBLEM: No TEMP record and _measurement_temperature .NE.        293 Degree
RESPONSE: The alert arises due to the low temperature (100 k) data collection.
;
_vrf_PLAT972_c2byc_a             
;
PROBLEM: Check Calcd Resid. Dens.  0.86Ang From U5             -3.20 eA-3  
RESPONSE: The alert arises due to the strong absorptions for heavy U atoms.
;
# end Validation Reply Form
